Research Article  Open Access
Micromagnetic Investigation of Periodic CrossTie/Vortex Wall Geometry
Abstract
A systematic series of micromagnetic simulations on periodic crosstie/vortex wall structures in an ideal soft film at various widths, thicknesses, and period lengths is performed. For each width and thickness a natural period length is found which has minimal energy density for walls of this type. For each width, a critical thickness is determined below which the natural period length is infinite; for films thinner than this, the pure Néel wall has lower energy than any crosstie/vortex wall. Details of the origin of the energy reduction in crosstie/vortex walls as compared to Néel walls are also examined, and canting inside crosstie and vortex structures in films thicker than 1 is explained.
1. Introduction
The predominant types of domain walls in soft films are Néel walls occurring in very thin films, Bloch walls in thicker samples, and numerous transitional structures [1–3]. One of the more interesting transitional structures is the crosstie/vortex (or simply crosstie) wall which alternates crossties and vortices between counterrotating segments of Néel walls. Crosstie/vortex walls are observed experimentally [4–6], in micromagnetic simulations [6–9], and in theory [10, 11]. In finite samples, this wall type appears in low remanence closedflux Landau patterns, as seen in Figure 1. If the structure is long enough, then multiple crossti/evortex pairs can appear, as in Figure 2.
To gain insight into the formation and structure of crosstie/vortex walls, this work presents a systematic collection of micromagnetic simulations performed using the OOMMF micromagnetic package from NIST [12]. An ideally soft material was modeled (anisotropy constant J/m^{3}) with saturation magnetization kA/m and exchange coefficient pJ/m, to approximate an NiFe alloy. All of the simulations were performed with no applied field.
The component energies in this system are the stray field energy and the exchange energy, with the component fields defined by: where is the normalized (unit) magnetization. In both cases, energy density , where the factor arises from the dependence of on . Thus the total energy density in the system is
In soft films, the relevant length scale is the magnetostaticexchange length, defined by where is the magnetostatic energy density All lengths reported herein are in units of , and energy densities are reported in units of . However, for the given values of and , nm and kJ/, so the results may be easily converted to nm and J/ if desired.
2. Simulation Details
Aside from Figures 1 and 2, the simulations in this paper are periodic along the long axis of the wall, as indicated in Figure 3. This allows the structure of the crosstie/vortex wall to be studied separately from the effects of edge domains. The period length is denoted by , with and denoting the sample width and thickness, respectively. Coordinates are introduced such that positions inside the simulation volume run from , , and .
The computational cells are approximately cubic in shape, with each edge dimension not larger than . This size is small enough that the maximum change in magnetization angle from one cell site to the next is kept below about ; this suffices to provide a good rendering of the magnetization on the discretized grid. The and cell sizes are adjusted downward if necessary to make the count of cells across each of the and dimensions odd, so that there is a unique center cell along each of those dimensions. The cell size is adjusted downward as necessary so that the count of cells along the dimension is (so allowed cell counts are 2, 6, 10,). Taken together, these adjustments allow a unique cell in the center of each of the vortex and crosstie cores to be identified.
The initial magnetization configuration for each simulation is either taken from the end state of a previous run (if one is available that is close to the dimensions of the current run) or else set to a cartoon version of the crosstie/vortex configuration as illustrated in Figure 3. Either way, the magnetization in the central cell in the vortex core is set to (along the film normal) and the central cell in the crosstie core is set to . Except as noted, the magnetization in these center cells is held fixed. As discussed in Rave [8], this pinning tends to accelerate convergence of simulations to equilibrium and improves accuracy. Simulations run without this constraint show no discernible difference in the end equilibrium state. Some simulations were also run with the vortex and crosstie cores both aligned in the direction. This raises the energy somewhat, but for most geometries the energy difference is negligible, typically less than one part in . For simulations with a period length to film thickness ratio of less that 10 : 1, however, the difference is larger. For example, in the , , case the energy in the aligned core setting was 3% larger than for the antialigned setting.
Once the initial magnetization is set, the simulation proceeds by energy minimization via a conjugategradient procedure, stopping when the reduced torque .
3. Results and Discussion
Each point in Figure 4 marks the average total energy density at equilibrium resulting from a simulation with width at the indicated thickness and period length . There is one crosstie/vortex pair in each period, so as the period length grows large the wall becomes primarily two Néel segments interrupted by a crosstie and vortex at either end. This is evident in the behavior of the curves for large , as for each thickness the curve asymptotically converges to the energy density of the associated Néel wall. For small period lengths () the energy density grows sharply as the exchange energy resists compression of the complex crosstie/vortex structure. For thinner films ( under about for ), the energy density curves are monotonically decreasing. This means that in a thin infinite strip if the crosstie and vortex are not pinned by some means, they will spread out indefinitely leaving behind a plain Néel wall. This is consistent with the experimental result that crosstie/vortex walls are not observed in ultrathin films. The transition thickness is a function of the strip width ; this dependence is explored in Figure 9 below.
For thicker films there is a unique minimum on each curve, which corresponds to a “natural” period length —this is the period length that minimizes the energy for a crosstie/vortex wall at the given film thickness and strip width. Note though that each point in Figure 4 is a stable equilibrium configuration under the fixed period assumption. So if the period length is constrained by geometry or other means such as pinning defects, then period lengths other than the natural length are possible, as seen in Figures 1 and 2.
The energy wells are asymmetric, especially for the midlevel thicknesses, say between and . In this regime the penalty for a period longer than the natural period is small, but in all cases periods significantly shorter than the natural period are energetically prohibitive.
Another feature of the curves in Figure 4 is that as the films grow thicker, the energy density increases, the natural period length grows shorter, and the energy well is deeper. These effects can be explained by examining the stray field and exchange component energies of the total energy.
In this regard, note two attributes of the magnetization in these simulations. The first is that the shape anisotropy of thin films constrains the magnetization to lie mostly inplane (the notable exception being of course the cores of vortex and crosstie structures). The second is that the magnetization does not vary much along the film normal () direction. This is due in part to the dominance of exchange coupling over the relatively short distance between the top and bottom of each film and also due to the relative uniformity of stray field in . (The latter condition does not hold near the vicinity of the vortex and crosstie cores, and this leads to nearby variation in , as will be seen below.)
The second attribute means we can meaningfully consider a situation where the magnetization is held fixed and the thickness of the part is varied. In this setting the first integral in the formula for the stray field (1), which handles the effects of the bulk charge, is seen to vary linearly with thickness via the change in the part volume. Ignoring magnetic charges on the top and bottom surfaces in the second integral, we see that it too varies linearly with (although in the Landau fluxclosure structures considered here this contribution is minor regardless). The net result is that if the magnetization were held fixed, then reducing the film thickness would be expected to reduce the stray field by a similar amount. The exchange field (2), however, does not vary with thickness . This means that one can expect exchange to take on a more dominant role as the film thickness is decreased.
These effects are on display in Figure 5, which breaks down the total energy density curves from Figure 4 for two thicknesses into the stray field and exchange components. For both thicknesses we see the dominance of the exchange energy in shortperiod lengths, giving way to the stray field energy for longer period lengths. Moreover, for each component the energy density is greatly reduced in the thinner strip. If the magnetization configurations were the same for the two thicknesses, then by the above analysis the exchange energy density would stay constant and the stray field energy density would drop by a factor of six. In practice, of course, what happens is that the weak stray field in the thinner film allows the magnetic structures to expand, reducing the exchange energy at the expense of a modest increase in the stray field.
To understand how crosstie/vortex structures lower the energy density of a Néel wall, return to Figure 1, and focus first on a section of the Néel portion of the wall between the left hand vortex and the crosstie. Moving from bottom to top across the wall, the magnetization rotates counterclockwise. This configuration produces negative magnetic charge on the lower half of the strip (dark region) and positive charges on the upper half (light region). (Here “lower” and “upper” refer to the view on the page.) This sets up a stray field running from the positive charges to the negative charges, counter to the magnetization in the center of the wall, making the wall center a high stray field energy density region. On the right hand side of the crosstie the magnetization rotation direction across the wall is reversed, so that the positive charge region is below the wall and the negative charge region is above. The wall is still a high stray field energy density region, but the checkerboarding of the charge regions reduces the total stray field energy in two ways. The first factor is that by effectively arranging the charge regions into a quadrupole configuration, the extent of their stray field is reduced. The second, larger contribution is seen more clearly in Figure 2. In the checkerboard pattern, stray field between the charge blocks runs not only up and down across the Néel sections of the wall, but also left and right horizontally parallel to the wall. The orientation of the magnetization about each vortex core is such that it aligns with the stray field from the nearby charge blocks, so that the regions above and below each vortex are regions of low stray field energy density.
This latter effect is shown directly in Figure 6, which is from the (periodic) simulation corresponding to the minimum point on the curve in Figure 4. Parts (b)–(d) of this figure are shaded to indicate the component and total energy densities as a function of position. In part (b), the lightcolored low energy density regions above and below the vortex core are clearly visible. Part (c) shows the regions of high exchange energy density. These include the vortex core and center of the wall, as expected. It is interesting that there is also a region of high exchange energy running perpendicular to the wall through the crosstie core. In an idealized crosstie, the magnetization rotates around the crosstie core in the same manner as the magnetization rotates about a vortex core, only with the opposite winding number. In such a configuration the exchange energy is exactly the same as for a vortex (the stray field energy is a different matter, of course), so the high exchange energy spike perpendicular to the wall must arise due to deformation of the crosstie structure. Most likely the observed buckling in the magnetization along this line is caused by the horizontal stray field from the checkerboard charge regions which flows counter to the magnetization here.
(a)
(b)
(c)
(d)
Additional details may be gleaned from Figure 7, which shows crosssectional averages for Figure 6 and includes a blackdashed line showing the energy density for a pure Néel wall in this geometry. The energy savings in stray field energy around the vortex core, and expense around the crosstie core, are shown by the green line. On either side of the crosstie and vortex cores, the magnetization spreads out slightly as compared to a Néel wall, and as a result the exchange energy density (blue line) in those regions is slightly less than the exchange energy density for a Néel wall (not shown). This savings is more than offset by the increase in exchange energy inside the vortex and crosstie core structures, so that in total the exchange energy for the crosstie/vortex wall is higher than the exchange energy for the Néel wall. (Another view of this is that the wall structure outside the cores is essentially that of a stretched Néel wall; the stretching reduces the exchange energy, but the stray field energy across the wall is increased by more than the exchange energy reduction.) The dashed red line shows the combined (stray field plus exchange) energy density averaged across each half of the simulation volume. This shows a clear reduction in energy density as compared to the Néel wall for the portion of the simulation about the vortex, and a clear increase about the crosstie. The average of these two halflines is the average energy density for the crosstie/vortex wall as a whole, which is slightly below the energy density for the pure Néel wall. An important point here is that the crosstie structure by itself costs energy as compared to the Néel wall; the crosstie/vortex wall formation as a whole is energetically favorable only because of the stray field energy savings associated with the vortex structure.
The two graphs, Figures 8 and 9, collect information on the natural period lengths from Figure 4 and similar simulation series for several other strip widths. For each strip width and thickness , a sequence of simulations was performed using a golden section search to locate the precise period that minimized the total energy density. In Figure 8 we observe that for each strip width , the minimal period length data can be fitted fairly well by a curve of the form , where is the film thickness and , , and are fit parameters. In this fit only the data for are used; in the thicker films the crosstie and vortex structures develop significant asymmetry which alters the character of the structure. If this asymmetry did not develop, then the parameter would describe the asymptotic period length that would be obtained in thick films.
At the other end of the scale, we see that each of the curves in Figure 8 has a pole on the left, which corresponds to parameter . As discussed above with respect to the curve in Figure 4, if a film is thin enough then there is no minimal period length. For each strip width , the critical thickness dividing the two regimes corresponds to the location of the pole in Figure 8 (or, equivalently, parameter ). The critical thickness as a function of strip width is plotted on a loglog scale in Figure 9. We see from the fitted curve, , that the critical thickness decreases with increasing strip width. From a practical standpoint the natural period length can be quite large. For example, although the curve in Figure 4 appears to be monotonically decreasing, the fit in Table 1 predicts a minimum at , or roughly m in NiFe.

As an example of the use of Figure 8, refer again to the finite system of Figures 1 and 2. If we allow for a border at each of the left and right sides of the sample to accommodate edge closure domains, then that leaves a run in the middle for the crosstie/vortex wall. From Figure 8, we see that the natural period length for a strip of width and thickness is just under . This predicts that a configuration with four crosstie/vortex periods would have lower energy than either the three period configuration shown in Figure 2 or a five period configuration. Direct simulations on the finite system bear out this result.
In regions where the magnetization lies inplane, the stray field is nearly uniform through the thickness of the film, and so the magnetization also shows little variation in . The vortex and crosstie core regions, however, are delineated by outofplane magnetization, and this does produce a dependence on the magnetization near the cores. This effect is shown in Figures 10 and 11. (For this simulation, the magnetization in the central cells of the cores was not pinned.) Looking first at the magnetization at the top surface around the vortex core (Figure 10(a)), the magnetization in the vortex core points out of the plane, and the resulting positive magnetic charge interacts with the checkerboard magnetic charge pattern on either side by pushing the positive charge blocks away (towards on the left and on the right) and extending the negative charge regions. This causes a “microdeformation” of the wall [7]; the spacing between the arrows in the diagram is roughly , so the total deformation is about . Outside the viewed region, at about on either side of the core, the wall shifts back to the center line.
(a)
(b)
(c)
(d)
(a)
(b)
(c)
(d)
On the bottom surface of the film (Figure 10(c)), the surface charge from the core has the opposite charge, and the wall shifts in the opposite direction, while the midplane shows no shift at all (Figure 10(b)). A crosssection through the thickness of the film (Figure 10(d)) shows that the wall is actually canted by about from the vertical. Outside of this view area, the Néel portions of the wall are not canted, but run through the thickness of the film independent of . Figure 11 shows that the magnetization around the crosstie core behaves similarly.
This effect relies on the opposite charges on the top and bottom surfaces being sufficiently far apart that they can independently influence the nearby magnetization. For thinner films, the extent of the dipole field from the core diminishes relative to the exchange length and the wall canting is reduced; for films thinner than about the effect is not evident.
4. Conclusion
In an ideally soft magnetic thin film, the crosstie/vortex wall is a periodic structure consisting of alternating crossties and vortices sandwiched between Néel wall segments having alternating chiralities. This structure is primarily two dimensional (i.e., independent of ), with the exception of minor canting on either side of both crosstie and vortex cores in films thicker than .
In an infinite strip, the crosstie/vortex wall structure has a natural period length that minimizes the energy density for this class of walls, and this length is a function of both the strip thickness and width. For a given strip width , there is a critical thickness below which the natural period length is infinite. That relation is , with and measured in . In films thicker than , the energy reduction obtained by a crosstie/vortex wall as compared to a plain Néel wall is the result of decreased stray field energy across the outboard sides of the vortex cores arising from the checkerboarding of the magnetic charge associated with the Néel wall segments.
Related periodic wall structures are topologically permissible, for example one could replace each vortex in the crosstie/vortex structure with a counterrotating crosstie, or replace each crosstie with a counterrotating vortex. The former is probably energetically illfavored, but the latter produces the wellknown diamond state that frequently sports lower energy than the crosstie/vortex wall [8].
References
 R. Kirchner and W. Döring, “Thin films: domain walls and related topics,” Journal of Applied Physics, vol. 39, pp. 855–856, 1968. View at: Google Scholar
 D. V. Berkov, K. Ramstöck, and A. Hubert, “Solving micromagnetic problems. Towards an optimal numerical method,” Physica Status Solidi, vol. 137, pp. 207–225, 1993. View at: Google Scholar
 K. Ramstöck, W. Hartung, and A. Hubert, “The phase diagram of domain walls in narrow magnetic strips,” Physica Status Solidi, vol. 155, no. 2, pp. 505–518, 1996. View at: Google Scholar
 R. Ploessl, J. N. Chapman, A. M. Thompson, J. Zweck, and H. Hoffmann, “Investigation of the micromagnetic structure of crosstie walls in permalloy,” Journal of Applied Physics, vol. 73, no. 5, pp. 2447–2452, 1993. View at: Publisher Site  Google Scholar
 A. Hubert and R. Schäfer, Magnetic Domains, Springer, 1998.
 S. Hou, G. Pan, D. J. Mapps et al., “Magnetic force microscopy and micromagnetic study of crosstie wall structures in Co_{91}Nb_{6}Zr_{3} amorphous thin films,” Journal of Applied Physics, vol. 87, no. 3, pp. 1096–1102, 2000. View at: Google Scholar
 M. Redjdal, A. Kakay, M. F. Ruane, and F. B. Humphrey, “Crosstie walls in thin permalloy films,” IEEE Transactions on Magnetics, vol. 38, no. 5, pp. 2471–2473, 2002. View at: Publisher Site  Google Scholar
 W. Rave and A. Hubert, “Magnetic ground state of a thinfilm element,” IEEE Transactions on Magnetics, vol. 36, no. 6, pp. 3886–3899, 2000. View at: Publisher Site  Google Scholar
 R. Hertel, “Thickness dependence of magnetization structures in thin Permalloy rectangles,” Zeitschrift für Metallkunde, vol. 93, no. 10, pp. 957–962, 2002. View at: Google Scholar
 F. Alouges, T. Rivière, and S. Serfaty, “Néel and crosstie wall energies for planar micromagnetic configurations,” ESAIM, vol. 8, pp. 31–68, 2002. View at: Publisher Site  Google Scholar
 A. DeSimone, H. Knüpfer, and F. Otto, “2d stability of the Néel wall,” Calculus of Variations and Partial Differential Equations, vol. 27, no. 2, pp. 233–253, 2006. View at: Publisher Site  Google Scholar
 M. J. Donahue and D. G. Porter, “OOMMF user’s guide, version 1.0,” NISTIR 6376, National Institute of Standards and Technology, Gaithersburg, Md, USA, 1999. View at: Google Scholar
Copyright
Copyright © 2012 Michael J. Donahue. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.